nanoparticles that were transfected with a gene that promotes wound healing and inhibits corneal fibrosis. Toxicity due to size of nanoparticles Toxicity in certain systems can also be dependent on the size of the nanoparticle. AuNSs size 1.4 nm were found to be toxic in human skin cancer cells (SK-Mel-28), human cervical cancer cells (HeLa), mouse fibroblast cells (L929), and mouse macrophages (J774A.1), while 0.8, 1.2, and 1.8 nm sized AuNSs were less toxic by a six-fold amount and 15 nm AuNSs were nontoxic. There is some evidence for AuNP buildup after injection in in vivo studies, but this is very size dependent. 1.8 nm AuNPs were found to be almost totally trapped in the lungs of rats. Different sized AuNPs were found to buildup in the blood, brain, stomach, pancreas, kidneys, liver, and spleen. Biosafety and biokinetics investigations on biodegradable ultrasmall-in-nano architectures have demonstrated that gold nanoparticles are able to avoid metal accumulation in organisms through escaping by the renal pathway. Synthesis Generally, gold nanoparticles are produced in a liquid ("liquid chemical methods") by reduction of chloroauric acid ().To prevent the particles from aggregating, stabilizing agents are added.Citrate acts both as the reducing agent and colloidal stabilizer. They can be functionalized with various organic ligands to create organic-inorganic hybrids with advanced functionality. Turkevich method This simple method was pioneered by J. Turkevich et al. in 1951 and refined by G. Frens in the 1970s. It produces modestly monodisperse spherical gold nanoparticles of around 10–20 nm in diameter.Larger particles can be produced, but at the cost of monodispersity and shape. In this method, hot chloroauric acid is treated with sodium citrate solution, producing colloidal gold. The Turkevich reaction proceeds via formation of transient gold nanowires. These gold nanowires are responsible for the dark appearance of the reaction solution before it turns ruby-red. Capping agents A capping agent is used during nanoparticle synthesis to inhibit particle growth and aggregation. The chemical blocks or reduces reactivity at the periphery of the particle—a good capping agent has a high affinity for the new nuclei. Citrate ions or tannic acid function both as a reducing agent and a capping agent. Less sodium citrate results in larger particles. Brust-Schiffrin method This method was discovered by Brust and Schiffrin in the early 1990s, and can be used to produce gold nanoparticles in organic liquids that are normally not miscible with water (like toluene). It involves the